Antibacterial Activity of ZnSe, ZnSe-TiO2 and TiO2 Particles Tailored by Lysozyme Loading and Visible Light Irradiation

ZnSe, ZnSe-TiO2 microspheres and nanostructured TiO2 obtained by hydrothermal and sol–gel methods were tested against Staphylococcus aureus ATCC 25923 and Micrococcus lysodeikticus ATCC 4698 before and after lysozyme (Lys) loading. Morphological characterization of inorganic matrices and hybrid organic–inorganic complexes were performed by microscopy techniques (SEM, AFM and Dark Field Hyperspectral Microscopy). Light absorption properties of ZnSe, ZnSe-TiO2 and TiO2 powders were assessed by UV–visible spectroscopy and their ability to generate reactive oxygen species (•OH and O2•−) under visible light irradiation was investigated. Antibacterial activity of ZnSe, ZnSe-TiO2, TiO2, Lys/ZnSe, Lys/ZnSe-TiO2 and Lys/TiO2 samples under exposure to visible light irradiation (λ > 420 nm) was tested against Staphylococcus aureus and Micrococcus lysodeikticus and correlated with ROS photogeneration.


Introduction
In the last years, a large range of engineered materials have been studied in order to develop new antibacterial tools meant to support healthcare and life quality due to the excessive use of chemicals and antibiotics producing major imbalances in the beings' behavior. Therefore, it is mandatory now to find new pathways able to limit the aggression of pathogens and their increasing resistance. For instance, the intensive use of biologically active compounds (antibacterial enzymes, antibodies and biological markers) [1,2] for biomedical application can be a useful approach since their drawbacks (high costs and short lifetime) are already known and can be overcome by embedding them in hybrid organic-inorganic systems with increased activity, reusability and higher endurance [3,4]. These should also contain valuable inorganic materials only for carrying the bioactive compounds or endow themselves with intrinsic antibacterial properties. The lysozyme (1,4-N-acetylmuramidase) is such a biologically active compound and an antibacterial enzyme present in the living world and human body causing cell wall lysis in Gram-positive bacteria. It is largely studied [5] both for its antibacterial and enzymatic properties [6][7][8] but also for its interactions in different media, such as model protein [9,10].
The bioactivity of synthetic inorganic materials was deeply investigated, with many studies focusing on SiO 2 and TiO 2 [11] obtained by the sol-gel method because it uses materials that are non-toxic, low cost and well-investigated, but many other inorganic (a) Through formation of a hybrid complex by lysozyme loading (Lys/ZnSe, Lys/ZnSe-TiO 2 and Lys/TiO 2 ); (b) By exposing the light sensitive samples (ZnSe, ZnSe-TiO 2 and TiO 2 ) and their hybrid complexes (Lys/ZnSe, Lys/ZnSe-TiO 2 and Lys/TiO 2 ) to visible light irradiation before the antibacterial assay on Staphylococcus aureus and Micrococcus lysodeikticus.
Photogeneration of reactive oxygen species (•OH and O 2 •− ) over the samples of interest is envisaged in order to depict the particularities of the antibacterial mechanism for each sample. The effect of Lys/ZnSe-TiO 2 on Staphylococcus aureus was also monitored by Dark field microscopy and the morphological particularities of lysozymes, Staphylococcus aureus and Micrococcus lysodeikticus before and after interaction with the investigated samples by atomic force microscopy.
For a valid comparison between the investigated materials and their properties, the TiO 2 sample studied in this work was subjected after sol-gel synthesis to the same hy-drothermal treatment (aqueous hydrazine and NaOH media) as in the case of ZnSe and ZnSe-TiO 2 samples.

Lysozyme Adsorption on ZnSe, ZnSe-TiO 2 and TiO 2 Samples
Lysozymes (obtained from chicken egg white) and potassium phosphate buffer solution (PBS, pH 6.5) were provided by Lysozyme Activity Kit-LY0100 Sigma Aldrich (Sigma, Product of USA, St Luis). A total of 0.01 g of ZnSe, ZnSe-TiO 2 and TiO 2 powders were dispersed in 10 mL PBS containing lysozyme (0.25 mg/mL) and then gently shaken for 4 h at 25 • C. The solid samples were recovered by centrifugation (10,000 rpm for 10 min), washed with PBS/ultrapure water and dried at vacuum for further investigation, such as AFM and antibacterial characterization. Supernatants containing lysozyme were characterized by UV-visible spectroscopy. Additionally, the PBS containing lysozyme sand Micrococcus lysodeikticus ATCC 4698 0.01% w/v (Lysozyme Activity Kit-LY0100 Sigma Aldrich) was used for preparation of AFM samples by drop-casting on Si or glass substrates.

Scanning Electron Microscopy (SEM)
SEM images have been obtained using a high-resolution microscope, Quanta 3D (FEI, Eindhoven, The Netherlands) at operating voltages between 5 and 20 kV.

Dark field microscopy
Dark field hyperspectral microscopy characterization was carried out using a Cyto Viva Hyperspectral Microscope in order to capture optical and hyperspectral images of Staphylococcus aureus in the presence of the lysozyme/ZnSe-TiO 2 complex. In this sense, S. aureus cell suspension (prepared according to Antibacterial assay section) was exposed for 4 h to lysozyme/ZnSe-TiO 2 and maintained at 37 • C by using a shaker incubator. A droplet of the sample was applied and left to dry on a microscope slide.

Atomic force microscopy (AFM)
Atomic force microscopy (AFM) measurements were made in non-contact mode with XE-100 from Park Systems. XE100 (Park Systems, Suwon, Republic of Korea) microscope used flexure-guided, crosstalk eliminated scanners thus minimizing the tip-sample interaction. All AFM images were recorded with sharp tips, NCHR-type (Nanosensors TM ), of less than 10 nm radius of curvature (typically 8 nm),~125 µm length,~30 µm width,~42 N/m force constant and~330 kHz resonance frequency. The AFM images were processed with XEI program (v 1.8.0-Park Systems) for displaying purpose and roughness evaluation. In order to improve the topographic details, the images are presented in so-called "enhanced contrast" view mode. This is a peculiarly colored view mode patented by Park Systems used to enhance the morphological characteristics, which employ the change of a pixel relative to its neighbors. Representative line scans are showed below 2D AFM images, which present in detail the surface profile of the scanned samples. The root-mean-squared roughness (Rq) represents the standard deviation of the height value in the image, while the peak-to-valley parameter (Rpv) is the height difference between the lowest and the highest points [27].

Diffuse Reflectance UV-Vis
UV-visible spectra were obtained with a Perkin Elmer Lambda 35 spectrophotometer equipped with an integrating sphere. Using the Kubelka-Munk function, the recorded reflectance data were changed into absorption spectra.

Reactive Oxygen Species (ROS) Generation under Visible Light Irradiation
Hydroxyl radicals (•OH) assessment In order to evaluate the hydroxyl radical's production (•OH), a coumarin solution (10 mM, Merck) containing 0.001 g of suspended powder (inorganic and hybrid complex) was irradiated with visible solar light (Peccel Solar Simulator, Japan, equipped with a cutoff filter λ > 420 nm, Asahi Spectra). The spectrum of the illumination source is provided in Supplementary Information (Figure S1). The fluorescent umbelliferone resulted from coumarin interaction with the photogenerated hydroxyl radicals and was further monitored with a Carry Eclipse fluorescence spectrometer, Agilent Technologies, (slits set to 5/10 nm in excitation and emission) for λ exc = 330 nm.
2.3.6. X-ray Fluorescence (XRF) Characterization for Ion Releasing Measurements XRF was used for elemental analysis of the liquid collected after a dialysis process involving the suspended powders in water (ZnSe, ZnSe-TiO 2 , TiO 2 , Lys/ZnSe, Lys/ZnSe-TiO 2 and Lys/TiO 2 ). In this sense, 0.03 g of each material was dispersed in 2 mL ultrapure water (Millie-Q system, >18 MΩcm), put in a dialysis bag (ZelluTrans/Roth regenerated cellulose membrane with wall thickness of 28 µm) and immersed in 5 mL ultrapure water, (Millie-Q system) contained by a glass beaker. The suspension was gently shaken with a magnetic stirrer for 24 h at room conditions. The system was adapted after Balint et al. [28]. Aliquots from the dialyzed liquid were subjected to XRF analysis looking for the released ions (presumable zinc, selenium and titanium ions). The measurements were performed using a Rigaku ZSX Primus II spectrometer (Rigaku Corp., Tokyo, Japan), equipped with 4.0 kW X-ray Rh tube. EZ-scan combined with Rigaku SQX fundamental parameters software (standard less) was used for data analysis.
For the liquid samples, the droplet method was used. Droplet method (or filter paper method) is used for analysis of the dried droplet solution on special filter paper [29].
2.4. Antimicrobial Activity Assay 2.4.1. Antimicrobial Activity Assay for the Inorganic Samples (ZnSe, ZnSe-TiO 2 and TiO 2 ) and Their Hybrid Complex with Lysozyme (Lys/ZnSe, Lys/ZnSe-TiO 2 and Lys/TiO 2 ) Staphylococcus aureus ATCC 25923 (American Type Culture Collection) and Micrococcus lysodeikticus ATCC 4698 lyophilized cells (from Lysozyme Activity Kit-LY0100 Sigma Aldrich) were used as model organisms to evaluate the antibacterial activity of target materials. The reference strains were grown overnight on TSB (Tryptic Soy Broth, Scharlab, Spain) at 37 • C. The antibacterial potential was assessed based on the pour plate method. The fresh bacterial inoculum was suspended in 0.85% NaCl and the turbidity was adjusted to 10 8 colony-forming units per milliliter (CFU/mL), corresponding to 0.5 Mc Farland standard, according to CLSI (Clinical and Laboratory Standards Institute). The standardized bacterial suspension was inoculated into TSB and incubated for four hours at 37 • C with 150 rpm shaking in the presence of 0.01 g of the synthesized samples. Subsequently, 10-fold serial dilutions were performed from the obtained suspension and appropriate volumes of diluted samples were spread on TSA (Tryptic Soy Agar, Scharlab, Spain) plates and incubated at 37 • C for 24 h. The number of colonies were counted and the results were expressed as CFU/mL (colony-forming unit per mL). The percentage of cell survival was calculated based on the control sample represented by the untreated bacterial culture. Experiments were performed in triplicate.
2.4.2. Antimicrobial Activity Assay for the Samples of Interest Assisted by Visible Light Irradiation (λ > 420 nm) The antibacterial activity of the synthesized materials was tested against the reference bacterial strains Staphylococcus aureus ATCC 25923 and Micrococcus lysodeikticus ATCC 4698. Cells were grown overnight at 37 • C with 150 rpm shaking by inoculating a bacte- rial single colony in TSB. A bacterial suspension obtained in MilliQ sterile water with a concentration of 10 5 colony-forming units per milliliter (CFU/mL) was used for the antibacterial experiment. The efficacy of the samples against bacterial suspension was assessed in a sterile 96-well plate. A total of 0.01 g from the investigated materials (ZnSe, ZnSe-TiO 2 , TiO 2 , Lys/ZnSe, Lys/ZnSe-TiO 2 and Lys/TiO 2 ) was placed in each well, over which 20 µL of standardized bacterial suspension was added and irradiated with visible light (λ > 420 nm) for 10, 20 and 30 min. Subsequently, fresh liquid culture medium was added to each sample well. A serial decimal dilution in a sterile saline solution was performed and plated onto TSA. The number of colonies was counted after 24 h of incubation at 37 • C and expressed as CFU/mL. A control sample, represented by the irradiated bacterial suspension without materials of interest, was also prepared. The percentage of cell survival was calculated. Experiments were performed in triplicate. After 30 min of light exposure, 3 µL of each bacterial suspension containing ZnSe, ZnSe-TiO 2 , TiO 2 , Lys/ZnSe, Lys/ZnSe-TiO 2 and Lys/TiO 2 was extracted and deposited on glass substrate (Heinz Herenz, Hamburg, Germany) for AFM analysis.

Scanning Electron Microscopy (SEM)
SEM images of the ZnSe, ZnSe-TiO 2 and TiO 2 samples were presented in Figure 1, which shows that nanoparticles assembled as micrometer-sized spheres for ZnSe-based materials and aggregates of nano-scaled particles for TiO 2 . A perceivable surface roughness and incipient exfoliation process can be observed for ZnSe spheres (Figure 1a,b), whereas for the composite material (ZnSe-TiO 2 ), smaller and closely packed particles can be depicted at the surface of microspheres with disposition for gathering (Figure 1c,d).
Antioxidants 2023, 12, x FOR PEER REVIEW 5 of 24 appropriate volumes of diluted samples were spread on TSA (Tryptic Soy Agar, Scharlab, Spain) plates and incubated at 37 °C for 24 h. The number of colonies were counted and the results were expressed as CFU/mL (colony-forming unit per mL). The percentage of cell survival was calculated based on the control sample represented by the untreated bacterial culture. Experiments were performed in triplicate.

Antimicrobial Activity Assay for the Samples of Interest Assisted by Visible Light Irradiation (λ > 420 nm)
The antibacterial activity of the synthesized materials was tested against the reference bacterial strains Staphylococcus aureus ATCC 25923 and Micrococcus lysodeikticus ATCC 4698. Cells were grown overnight at 37 °C with 150 rpm shaking by inoculating a bacterial single colony in TSB. A bacterial suspension obtained in MilliQ sterile water with a concentration of 10 5 colony-forming units per milliliter (CFU/mL) was used for the antibacterial experiment. The efficacy of the samples against bacterial suspension was assessed in a sterile 96-well plate. A total of 0.01 g from the investigated materials (ZnSe, ZnSe-TiO2, TiO2, Lys/ZnSe, Lys/ZnSe-TiO2 and Lys/TiO2) was placed in each well, over which 20 μL of standardized bacterial suspension was added and irradiated with visible light (λ > 420 nm) for 10, 20 and 30 min. Subsequently, fresh liquid culture medium was added to each sample well. A serial decimal dilution in a sterile saline solution was performed and plated onto TSA. The number of colonies was counted after 24 h of incubation at 37 °C and expressed as CFU/mL. A control sample, represented by the irradiated bacterial suspension without materials of interest, was also prepared. The percentage of cell survival was calculated. Experiments were performed in triplicate. After 30 min of light exposure, 3 μL of each bacterial suspension containing ZnSe, ZnSe-TiO2, TiO2, Lys/ZnSe, Lys/ZnSe-TiO2 and Lys/TiO2 was extracted and deposited on glass substrate (Heinz Herenz, Hamburg, Germany) for AFM analysis.

Scanning Electron Microscopy (SEM)
SEM images of the ZnSe, ZnSe-TiO2 and TiO2 samples were presented in Figure 1, which shows that nanoparticles assembled as micrometer-sized spheres for ZnSe-based materials and aggregates of nano-scaled particles for TiO2. A perceivable surface roughness and incipient exfoliation process can be observed for ZnSe spheres (Figure 1a,b), whereas for the composite material (ZnSe-TiO2), smaller and closely packed particles can be depicted at the surface of microspheres with disposition for gathering (Figure 1c,d).
These morphological changes are induced by the presence of TiO2 at the surface of the composite material (ZnSe-TiO2), which been shown in our previous work [17]. This can trigger a specific antibacterial activity of the composite sample (ZnSe-TiO2) relative to the bare ones (ZnSe, TiO2). Figure 1e,f shows aggregates formed by TiO2 nanoparticles ranged between 50 and 100 nm.

Dark Field Microscopy (Cyto Viva)
Dark field microscopy was used for illustrating the interaction of Staphylococcus aureus with the lysozyme/ZnSe-TiO2 complex ( Figure 2).  These morphological changes are induced by the presence of TiO 2 at the surface of the composite material (ZnSe-TiO 2 ), which been shown in our previous work [17]. This can trigger a specific antibacterial activity of the composite sample (ZnSe-TiO 2 ) relative to the bare ones (ZnSe, TiO 2 ). Figure 1e,f shows aggregates formed by TiO 2 nanoparticles ranged between 50 and 100 nm.

Dark Field Microscopy (Cyto Viva)
Dark field microscopy was used for illustrating the interaction of Staphylococcus aureus with the lysozyme/ZnSe-TiO 2 complex ( Figure 2).

Dark Field Microscopy (Cyto Viva)
Dark field microscopy was used for illustrating the interaction of Staphylococcus aureus with the lysozyme/ZnSe-TiO2 complex ( Figure 2).   Figure 2a presents the bacterial morphology after its exposure to the Lys/ZnSe-TiO 2 complex (according to the Section 2.3.2). Additionally, in this image, the hybrid complex appears as a sparkling point due to the fluorescence of the lysozyme (containing the tryptophan residues) that surrounds the inorganic particle (ZnSe-TiO 2 ) and generates a core shell-type structure (this can be clearer depicted in Figure 2b, green circle) and is also proven in previous work [17]. Bacteria fragments can be observed in Figure 2a proving the harmful effect of Lys/ZnSe-TiO 2 on Staphylococcus aureus. The spectral comparison from Figure 2b certifies the contact of bacteria with the Lys/ZnSe-TiO 2 complex by providing the mean spectral profile for both lysozyme/ZnSe-TiO 2 (green signaled) and the Staphylococcus aureus/lysozyme/ZnSe-TiO 2 (red signaled) in the 400-1000 nm spectral range.
A mean region of interest (ROI) was captured from both samples. The data were then normalized to unity for comparison, being obvious that the lysozyme/ZnSe-TiO 2 hybrid complex and Staphylococcus aureus/lysozyme/ZnSe-TiO 2 exhibit a unique and distance spectral profile in the visible-NIR range (400-1000 nm), with the Staphylococcus aureus/lysozyme/ZnSe-TiO 2 having a peak location approximately 25 nm shifted to the right. Briefly, Figure 2a,b emphasizes the antibacterial effect of the lysozyme/ZnSe-TiO 2 complex against Staphylococcus aureus. In this sense, the effect may be attributed to the bacteria contact with lysozyme/ZnSe-TiO 2 (certified by Figure 2b), but other antibacterial mechanisms (ROS generation and ion releasing) can be envisaged. The foregoing antibacterial assay may add new data regarding the synergetic effects of lysozymes and ZnSe-TiO 2 .

Atomic force microscopy
Firstly, the AFM images were captured for TiO 2 nano-scaled particles supported on Si substrates alone and together with lysozyme (Lys) and Micrococcus lysodeikticus (MC), collected from buffered suspensions. Figures 3-6 contain AFM images recorded 48 h after the sample preparation.       marked by red circles in Figure 6. The MC pattern is even more recognizable at the scale of (2 μm × 2 μm), where diameters of ~200 nm are suggested by the corresponding line-scan from Figure 6c. At larger scales (4 μm × 4 μm and 8 μm × 8 μm-not shown here), MC bacteria with larger diameters (3-400 nm) are present on Lys/TiO2/Si. Taking into account that MC is deposited from buffered solution (not from bacterial inoculum) and the images were recorded after 48 h from deposition, these AFM images can be considered relevant for the MC interaction with lysozymes. The proper dimension of the MC will be revealed starting with Figure 8.  From the corrugation point of view, at the scale of (1 μm × 1 μm) (see Figure 6b), the MC/Lys/TiO2 deposited on Si(100) is characterized by the following roughness parameters: Rq = 6.50 nm and Rpv = 41.30 nm.
The roughness behavior of all scanned systems is summarized in Figure 7. It can be observed that the most corrugated surface is seen in the case of Lys deposited on Si due to the fibrillar-shaped particles and their agglomeration in the form of clusters.  The TiO 2 powder was imaged by dispersing it in water by ultrasonication (at a concentration of 0.5 mg/mL) and deposited on a clean Si(100) substrate. Figure 3 presents the morphology of the TiO 2 at the scale of (1 µm × 1 µm). From Figure 3, it can be observed that the TiO 2 powder prepared by sol-gel method plus further hydrothermal tratment exhibits a majority population of small hemi-spherical particles, with a main diameter around 50 nm and a tendency to form agglomerated particles with diameters up to hundreds of nm in diameter. The tendency for nanoparticles to agglomerate in spherical aggregates can also be noticed. At the scale of (1 µm × 1 µm), as exemplified in Figure 3, the TiO 2 particles deposited on Si(100) are characterized by the following roughness parameters: Rq = 6.51 nm and Rpv = 36.44 nm.
From Figure 4, two morphological characteristics can be observed for lysozymes deposited on Si, namely the quasi-spherical and fibrillar shaped species. More than that, it can be noticed that the features with a quasi-spherical (doughnut) appearance are composed of smaller entities, such as that marked between the two red arrows along the horizontal red line, with a diameter of~17.6 nm. On the other hand, the diameter of the fibrillar structure is~170 nm, as suggested by the vertical green line, while its length is~800 nm. Nevertheless, its texture suggests that the fiber is formed by the agglomeration of individual lysozymes. At the scale of (1 µm × 1 µm) ( Figure 4) the Lys/Si system is characterized by the following roughness parameters: Rq = 17.11 nm and Rpv = 122.34 nm. Figure 5 presents the AFM images obtained for the Lys/TiO 2 /Si system (resulted after the drop-casting deposition of lysozymes onto TiO 2 /Si specimens). From the 2D AFM images in Figure 5, it can be seen that lysozymes cover the TiO 2 particles exhibiting a strong tendency to form a network of inter-connected fibrils which are~6-8 nm in height. Random individual TiO 2 particles are still visible (some of them gathered in form of clusters-as seen in the corner left image of Figure 5b between the lysozyme fibers as well evidenced by the AFM image recorded at the scale of (2 µm × 2 µm) (Figure 5a). At the scale of (1 µm × 1 µm), as seen in Figure 5b, the Lys/TiO 2 particles deposited on Si(100) are characterized by the following roughness parameters: Rq = 4.24 nm and Rpv = 34.20 nm. The deposition of lysozymes takes place mainly on the TiO 2 particles, coating them and favoring fibrillar depositions.
Micrococcus lysodeikticus (MC) was added from buffered cell suspension to the lysozyme previously deposited on the TiO 2 /Si substrate resulting in the morphology presented in Figure 6 (MC/Lys/TiO 2 /Si). The previously formed network-like Lys/TiO 2 system that the MC bacteria it is disposed on top of, in the form of compact hills, can be seen marked by red circles in Figure 6. The MC pattern is even more recognizable at the scale of (2 µm × 2 µm), where diameters of~200 nm are suggested by the corresponding line-scan from Figure 6c. At larger scales (4 µm × 4 µm and 8 µm × 8 µm-not shown here), MC bacteria with larger diameters (3-400 nm) are present on Lys/TiO 2 /Si. Taking into account that MC is deposited from buffered solution (not from bacterial inoculum) and the images were recorded after 48 h from deposition, these AFM images can be considered relevant for the MC interaction with lysozymes. The proper dimension of the MC will be revealed starting with Figure 8.
From the corrugation point of view, at the scale of (1 µm × 1 µm) (see Figure 6b), the MC/Lys/TiO 2 deposited on Si(100) is characterized by the following roughness parameters: Rq = 6.50 nm and Rpv = 41.30 nm.
The roughness behavior of all scanned systems is summarized in Figure 7. It can be observed that the most corrugated surface is seen in the case of Lys deposited on Si due to the fibrillar-shaped particles and their agglomeration in the form of clusters.
The next set of AFM images were obtained by depositing a drop of suspension containing the bacterial inoculum (prepared according to Section 2.4.2) and inorganic matrices (TiO 2 , ZnSe-TiO 2 ) on clean microscopic glass substrates and measured after 1 h from specimen preparation. Figure 8 presents the MC bacteria from inoculum and TiO 2 deposited on glass.
From the corrugation point of view, at the scale of (1 μm × 1 μm) (see Figure 6b), the MC/Lys/TiO2 deposited on Si(100) is characterized by the following roughness parameters: Rq = 6.50 nm and Rpv = 41.30 nm.
The roughness behavior of all scanned systems is summarized in Figure 7. It can be observed that the most corrugated surface is seen in the case of Lys deposited on Si due to the fibrillar-shaped particles and their agglomeration in the form of clusters.  The next set of AFM images were obtained by depositing a drop of suspension containing the bacterial inoculum (prepared according to Section 2.4.2) and inorganic matrices (TiO2, ZnSe-TiO2) on clean microscopic glass substrates and measured after 1 h from specimen preparation. Figure 8 presents the MC bacteria from inoculum and TiO2 deposited on glass. The massive blocks represent the random disposed MC bacteria as having a particular texture. The red line suggests a diameter of ~500 nm, while the small particles are TiO2 with diameters one order of magnitude smaller (~50 nm, as suggested by the particle selected along the green line). At the scale of (2 μm × 2 μm) ( Figure 8) the MC/TiO2/glass sample is characterized by the following roughness parameters: Rq = 39.47 nm and Rpv = 172.75 nm. Figure 9 presents the MC bacteria with Lys/TiO2 deposited on glass at the scales of (6 μm × 6 μm) (Figure 9a) and (1 μm × 1 μm) (Figure 9b). The massive shape of the MC bacteria prevails over the morphology of Lys/TiO2, with the features selected along the red line being ~600 nm and along the vertical green line of approx. 400 nm. Nevertheless, the texture of MC is visible, and the dimensions are influenced by the presence of Lys/TiO2. At the scale of (2 μm × 2 μm), not shown here, the MC/Lys/TiO2/glass sample is The massive blocks represent the random disposed MC bacteria as having a particular texture. The red line suggests a diameter of~500 nm, while the small particles are TiO 2 with diameters one order of magnitude smaller (~50 nm, as suggested by the particle selected along the green line). At the scale of (2 µm × 2 µm) ( Figure 8) the MC/TiO 2 /glass sample is characterized by the following roughness parameters: Rq = 39.47 nm and Rpv = 172.75 nm. Figure 9 presents the MC bacteria with Lys/TiO 2 deposited on glass at the scales of (6 µm × 6 µm) (Figure 9a) and (1 µm × 1 µm) (Figure 9b). The massive shape of the MC bacteria prevails over the morphology of Lys/TiO 2 , with the features selected along the red line being~600 nm and along the vertical green line of approx. 400 nm. Nevertheless, the texture of MC is visible, and the dimensions are influenced by the presence of Lys/TiO 2 . At the scale of (2 µm × 2 µm), not shown here, the MC/Lys/TiO 2 /glass sample is characterized by the following roughness parameters: Rq = 73.36 nm and Rpv = 512.61 nm.      Finally, Figure 11 presents an AFM image of MC from inoculum with ZnSe-TiO 2 after 30 min of irradiation deposited on glass substrate, recorded at the scale of 2 µm × 2 µm. The image shows one massive MC bacterium with a diameter of~800 nm, which is surrounded by some random fragments resulting from the MC interaction with ZnSe-TiO 2 . The MC/ZnSe-TiO 2 sample is characterized by the following roughness parameters: Rq = 42.76 nm and Rpv = 221.41 nm. Finally, Figure 11 presents an AFM image of MC from inoculum with ZnSe-TiO2 after 30 min of irradiation deposited on glass substrate, recorded at the scale of 2 μm × 2 μm. The image shows one massive MC bacterium with a diameter of ~800 nm, which is surrounded by some random fragments resulting from the MC interaction with ZnSe-TiO2. The MC/ZnSe-TiO2 sample is characterized by the following roughness parameters: Rq = 42.76 nm and Rpv = 221.41 nm.
(a) (b) Figure 11. Two-dimensional AFM image of MC from inoculum with ZnSe-TiO2 after 30 min of irradiation, deposited on glass substrate, recorded at the scale of 2 μm × 2 μm (a), together with a characteristic line scan (b). Figure 12 presents the interaction of S. aureus bacteria (from inoculum) with TiO2 material after 30 min of irradiation. Figure 12a shows three S. aureus bacteria, the selected one having a diameter of ~410 nm, while Figure 12b catches an agglomeration of bacteria, the largest part being of ~777 nm (along the green line).
The S. aureus/TiO2 sample from Figure 12a is characterized by the following roughness parameters: Rq = 29.34 nm and Rpv = 181.22 nm. Figure 13 presents the interaction of S. aureus bacteria with ZnSe material after 30 min of irradiation. The image captured a bacterial agglomeration of approx. 656 nm (selected between two red arrows along the green line) nearby a ZnSe fragment. In the lower half of the image, some other bacterial fragments, separated or gathered, are visible. The S. aureus/ZnSe sample from Figure 13 is characterized by the following roughness parameters: Rq = 52.61 nm and Rpv = 371.41 nm.
Finally, Figure 14 presents AFM images recorded for S. aureus (from inoculum) interaction with ZnSe-TiO2 deposited on glass, after 30 min of irradiation, at the scale of (2 μm × 2 μm). The two AFM images captured distorted S. aureus bacteria with diameters from 428 nm (a) to 265 nm (b) after interaction with ZnSe-TiO2 material. The ZnSe-TiO2 is visible as fragments with a peculiar texture. Figure 14a is characterized by the following roughness parameters: Rq = 17.98 nm and Rpv = 120.79 nm.   Figure 12a shows three S. aureus bacteria, the selected one having a diameter of~410 nm, while Figure 12b catches an agglomeration of bacteria, the largest part being of~777 nm (along the green line).    Finally, Figure 14 presents AFM images recorded for S. aureus (from inoculum) interaction with ZnSe-TiO 2 deposited on glass, after 30 min of irradiation, at the scale of (2 µm × 2 µm). The two AFM images captured distorted S. aureus bacteria with diameters from 428 nm (a) to 265 nm (b) after interaction with ZnSe-TiO 2 material. The ZnSe-TiO 2 is visible as fragments with a peculiar texture. Figure 14a is characterized by the following roughness parameters: Rq = 17.98 nm and Rpv = 120.79 nm. For all samples deposited on glass, the roughness behavior of all scanned AFM images is summarized in Figure 15 showing that the most corrugated surface is observed for the MC/Lys/TiO2 system. For all samples deposited on glass, the roughness behavior of all scanned AFM images is summarized in Figure 15 showing that the most corrugated surface is observed for the MC/Lys/TiO 2 system.
(c) (d) Figure 14. Two-dimensional AFM images of S. aureus (from inoculum) with ZnSe-TiO2 deposited on glass substrate, after 30 min of irradiation, recorded in two areas at the scale of (2 μm × 2 μm) (a,b), with two characteristic surface profiles (c,d).
For all samples deposited on glass, the roughness behavior of all scanned AFM images is summarized in Figure 15 showing that the most corrugated surface is observed for the MC/Lys/TiO2 system.

UV-Vis Spectroscopy
The UV-visible analysis was performed on inorganic ZnSe, ZnSe-TiO2, TiO2 and lysozyme modified materials. The characterization of the inorganic samples was meant

UV-Vis Spectroscopy
The UV-visible analysis was performed on inorganic ZnSe, ZnSe-TiO 2 , TiO 2 and lysozyme modified materials. The characterization of the inorganic samples was meant to depict the light absorptive properties of the samples revealing their structural particularities. The spectra of interest were collected in the range of 200-800 nm ( Figure 16) and showed the higher light absorption intensity for the ZnSe-TiO 2 composite relative to the pristine samples, both in UV and visible domains. ZnSe material has the broad absorption band ranging between 400 and 600 nm. to depict the light absorptive properties of the samples revealing their structural particularities. The spectra of interest were collected in the range of 200-800 nm ( Figure 16) and showed the higher light absorption intensity for the ZnSe-TiO2 composite relative to the pristine samples, both in UV and visible domains. ZnSe material has the broad absorption band ranging between 400 and 600 nm.
Although the present TiO2 sample is in line with the TiO2 reference materials, having the absorption edge around 400 nm, it also displays a long and well-defined absorption tail in the visible range attributable to the generated surface defects during the post-synthesis thermal treatment.

ROS Generation under Visible Light Irradiation (λ > 420 nm)
Hydroxyl radical (•OH) generation was evaluated from PL emission at 451 nm for λexc = 330 nm, this being attributed to the formation of umbelliferone by the interaction of coumarin with the photogenerated •OH [30]. Figure 17a shows the ability of the ZnSe material to generate hydroxyl radicals under visible light irradiation that almost disappears when TiO2 is added to composite materials (Figure 17b). Although the present TiO 2 sample is in line with the TiO 2 reference materials, having the absorption edge around 400 nm, it also displays a long and well-defined absorption tail in the visible range attributable to the generated surface defects during the post-synthesis thermal treatment. Figure 16 reveals the UV-visible spectra for the hybrid complexes with lysozyme of the inorganic samples and the bare lysozyme. Although the decreasing absorbance is obvious for all the modified samples, Lys/ZnSe and Lys/ZnSe-TiO 2 still preserve light absorptive capacity in the visible range (400-600 nm).

ROS Generation under Visible Light Irradiation (λ > 420 nm)
Hydroxyl radical (•OH) generation was evaluated from PL emission at 451 nm for λ exc = 330 nm, this being attributed to the formation of umbelliferone by the interaction of coumarin with the photogenerated •OH [30]. Figure 17a shows the ability of the ZnSe material to generate hydroxyl radicals under visible light irradiation that almost disappears when TiO 2 is added to composite materials (Figure 17b).  The TiO 2 sample proves to be totally inactive to generate •OH radicals under visible light (Figure 17c), while the ZnSe-TiO 2 sample shows a very slight activity too. Figure 17 shows that the antibacterial mechanistic pathways of ZnSe sample may involve •OH. Figure 17d-f also present the formation of •OH radicals under visible light irradiation by the lysozyme modified samples, which appears to be sharply decreased for the ZnSe sample. On the contrary, the capacity of Lys/ZnSe-TiO 2 to generate •OH relative to the unmodified sample seems to be higher with a maximum centered at 451 nm appearing after 20 and 30 min of light exposure. In the case of the Lys/TiO 2 sample, this is missing.
The superoxide anion (O 2 •− ) formation was monitored following the intensity of the formazan characteristic peak (485 nm) [31]. Figure 18a,b displays broad absorption bands for ZnSe and ZnSe-TiO 2 samples that indicate presumable antibacterial effects due to the presence of O 2 •− . Conversely, the TiO 2 material shows a lack of activity. This could be related to the presence of surface defects induced by the hydrothermal treatment and the known TiO 2 inactivity in the visible range. Figure 17. Generation of hydroxyl radical by inorganic (a-c) and lysozyme modified materials (d-f) under visible light irradiation. For the lysozyme modified samples, a well-defined characteristic band with a maximum at 470 nm is displayed in the case of Lys/ZnSe-TiO2 and Lys/ZnSe. This certi- For the lysozyme modified samples, a well-defined characteristic band with a maximum at 470 nm is displayed in the case of Lys/ZnSe-TiO 2 and Lys/ZnSe. This certifies the production of O 2 •− despite the presence of adsorbed lysozyme on the inorganic surfaces. This seems to allow the electron trapping by the adsorbed oxygen.
3.6. Antimicrobial Activity Assay for the Inorganic Samples (ZnSe, ZnSe-TiO 2 , TiO 2 ) and Their Hybrid Complex with Lysozyme (Lys/ZnSe, Lys/ZnSe-TiO 2 and Lys/TiO 2 ) against S. aureus In order to determine the potential antimicrobial effect of the synthesized materials, we assessed the planktonic growth of microbial cells in the presence of investigated samples by using the viable cell count method. Our study showed that the planktonic growth of the S. aureus bacterial strain was influenced differently by the investigated samples as follows: it was significantly inhibited in the presence of ZnSe-based materials after four hours of exposure, as compared to the control sample but slightly affected by the presence of TiO 2 . Namely, a significant bacterium growth inhibition was observed when the cells were incubated in the presence of a ZnSe, ZnSe-TiO 2 and Lys/ZnSe-TiO 2 samples as reflected by the survival cell percentages (7.6%, 35.5%, and 2.2%, respectively) ( Figure 19). Surprisingly, the sample Lys/ZnSe proves to be inactive against S. aureus, but on the contrary, a beneficial effect of adding lysozymes to the ZnSe-TiO 2 sample is achieved.
In order to explain the strange behavior of the Lys/ZnSe sample, one of the most cited antibacterial mechanisms, namely the ion releasing, was investigated (according to Section 2.4) by X ray fluorescence measurements. Zinc ion release in solution through a dialysis membrane was proven only for the ZnSe sample. In the same experimental conditions, this is missing for the Lys/ZnSe and the other samples (Supplementary Materials Figure S2). This result could explain the lack of activity for the Lys/ZnSe sample if the ion release is considered the main degradative mechanism against S. aureus and for the high antibacterial activity of the bare ZnSe sample. It is likely that the lysozyme's presence at the ZnSe surface hinders the release of zinc ions in solution. Based on these results, different mechanisms (i.e., ROS generation) should be considered decisive for the antibacterial activity of the other samples. growth of the S. aureus bacterial strain was influenced differently by the investigated samples as follows: it was significantly inhibited in the presence of ZnSe-based materials after four hours of exposure, as compared to the control sample but slightly affected by the presence of TiO2. Namely, a significant bacterium growth inhibition was observed when the cells were incubated in the presence of a ZnSe, ZnSe-TiO2 and Lys/ZnSe-TiO2 samples as reflected by the survival cell percentages (7.6%, 35.5%, and 2.2%, respectively) ( Figure 19). Surprisingly, the sample Lys/ZnSe proves to be inactive against S. aureus, but on the contrary, a beneficial effect of adding lysozymes to the ZnSe-TiO2 sample is achieved. Figure 19. Survival cell percentage of S. aureus ATCC 25923 after four hours of exposure to synthesized materials. The data are presented as the mean of three independent measurements, with error bars representing the standard deviation of the mean.
In order to explain the strange behavior of the Lys/ZnSe sample, one of the most cited antibacterial mechanisms, namely the ion releasing, was investigated (according to Section 2.4) by X ray fluorescence measurements. Zinc ion release in solution through a dialysis membrane was proven only for the ZnSe sample. In the same experimental conditions, this is missing for the Lys/ZnSe and the other samples (Supplementary Materials Figure S2). This result could explain the lack of activity for the Lys/ZnSe sample if the ion release is considered the main degradative mechanism against S. aureus and for the high antibacterial activity of the bare ZnSe sample. It is likely that the lysozyme's presence at the ZnSe surface hinders the release of zinc ions in solution. Based on these results, different mechanisms (i.e., ROS generation) should be considered decisive for the antibacterial activity of the other samples.
The inhibition of ZnSe reactivity towards S. aureus induced by lysozyme loading was checked taking into account the different amounts of lysozyme: 0.01 g powder and 20 μL of initial lysozyme suspension added to ZnSe led to 90% cell survival; and 100% cell survival being obtained by increasing the amount of available lysozyme by ten and The inhibition of ZnSe reactivity towards S. aureus induced by lysozyme loading was checked taking into account the different amounts of lysozyme: 0.01 g powder and 20 µL of initial lysozyme suspension added to ZnSe led to 90% cell survival; and 100% cell survival being obtained by increasing the amount of available lysozyme by ten and fifty times. This particular behavior of Lys/ZnSe towards S. aureus needs to be closely investigated in a future dedicated study. fifty times. This particular behavior of Lys/ZnSe towards S. aureus needs to be closely investigated in a future dedicated study.

Antimicrobial Activity Assay for the Inorganic Samples (ZnSe, ZnSe-TiO2 and TiO2) and Their Hybrid Complex with Lysozyme (Lys/ZnSe, Lys/ZnSe-TiO2 and Lys/TiO2) against M. lysodeikticus
The antibacterial effects of the various synthesized materials were investigated by comparing the number of viable Micrococcus cells after being in contact with the target samples for four hours (Figure 20). Analyzing the data depicted in Figure 20, it can be observed that the number of viable Micrococcus cells considerably decreased in the presence of ZnSe and ZnSe-TiO2 samples when compared with the untreated sample, resulting in a bacterial reduction of 94.13% for ZnSe and 98.91% for ZnSe-TiO2. Viability was also impaired after four hours of incubation of the microbial cells in the presence of TiO2 (35.8% bacterial reduction) relative to the control cells.
Further analysis of the lysozyme loaded materials revealed their important role in the inhibition of microbial growth, displaying higher antibacterial activity than lysozyme-free samples. Figure 20 shows the decreasing (by 50%) viability M. lysodeikticus cells with lysozyme addition to the TiO2 relative to the bare sample.  Analyzing the data depicted in Figure 20, it can be observed that the number of viable Micrococcus cells considerably decreased in the presence of ZnSe and ZnSe-TiO 2 samples when compared with the untreated sample, resulting in a bacterial reduction of 94.13% for ZnSe and 98.91% for ZnSe-TiO 2 . Viability was also impaired after four hours of incubation of the microbial cells in the presence of TiO 2 (35.8% bacterial reduction) relative to the control cells.
Further analysis of the lysozyme loaded materials revealed their important role in the inhibition of microbial growth, displaying higher antibacterial activity than lysozyme-free samples. Figure 20 shows the decreasing (by 50%) viability M. lysodeikticus cells with lysozyme addition to the TiO 2 relative to the bare sample.
3.8. Antibacterial Activity of the Inorganic and Hybrid Materials (ZnSe, ZnSe-TiO 2 , TiO 2 Lys/ZnSe, Lys/ZnSe-TiO 2 and Lys/TiO 2 ) Exposed to Visible Light Irradiation against S. aureus and M. lysodeikticus A strong antibacterial effect against S. aureus (0% survival cell) after 10 min of visible light irradiation was registered for ZnSe, Lys/ZnSe, ZnSe-TiO 2 and Lys/ZnSe-TiO 2 materials (Figure 21a). These results can be correlated with Figure 17a,b,d,e and 18a,b,d,e that clearly indicate the ROS generation over ZnSe-based samples, especially over the unmodified ones (without lysozyme). Still, the formation of hydroxyl radicals over Lys/ZnSe-TiO 2 and the superoxide anion generation on both Lys/ZnSe and Lys/ZnSe-TiO 2 samples can explain the high antibacterial activity of the lysozyme-based complexes under light exposure. However, there is a high difference in microbial cell viability when comparing the ZnSe-based samples with the TiO 2 samples. The results revealed only a slight decrease in the bacteria reduction percentage (13.55%) compared with the control when the bacterium was exposed to the TiO 2 sample (Figure 21a). viability when comparing the ZnSe-based samples with the TiO2 samples. The results revealed only a slight decrease in the bacteria reduction percentage (13.55%) compared with the control when the bacterium was exposed to the TiO2 sample (Figure 21a).  Figure 21b illustrates the antibacterial activity of the investigated samples against M. lysodeikticus; a slight increase in the cell survival relative to S. aureus is noted. Additionally, by comparison with S. aureus, a stronger effect of adding lysozymes can be observed, especially for the TiO2 sample. The interaction of lysozyme modified samples with visible light appears to be beneficial for their antibacterial activity. All the above-mentioned re-  lysodeikticus; a slight increase in the cell survival relative to S. aureus is noted. Additionally, by comparison with S. aureus, a stronger effect of adding lysozymes can be observed, especially for the TiO 2 sample. The interaction of lysozyme modified samples with visible light appears to be beneficial for their antibacterial activity. All the above-mentioned results present the overall antibacterial response of the investigated materials, which are dependent on the surface chemistry of the inorganic samples, their capacity to load the lysozyme and activate it and also the specific interaction with bacteria. A previous study, regarding morphological and structural properties of ZnSe and ZnSe-TiO 2 [17], reported the presence of stilleite as single crystalline phase in a ZnSe sample and stilleite (ZnSe, 85%), zincite (ZnO, 3.3%) and anatase (TiO 2 , 11.9%) as crystalline components of a ZnSe-TiO 2 sample. Also, the specific surface area for ZnSe and ZnSe-TiO 2 was found to be 15 m 2 /g and 10. 94 m 2 /g, respectively, proving that the lysozyme loading capacity is slightly higher for ZnSe-TiO 2 samples than for ZnSe. The buffered powders of ZnSe and ZnSe-TiO 2 showed no significant differences in the electrokinetic potential (-18.65 mV for ZnSe and -17.95 mV for ZnSe-TiO 2 ); however, there was a shift toward positive values being obtained for their complexes with lysozyme [17]. Unlike ZnSe-based samples, the present TiO 2 material displayed a surface area of 130 m 2 /g (Supplementary Information, Figure S3) and a shift to more negative values after lysozyme loading (from −34.9 mV to −42.30 mV, Supplementary Information- Figure S4), which is not favorable to the electrostatic interaction with the negatively charged cell membrane. Despite the higher surface area of TiO 2 , this sample has a lower capacity to load lysozyme than ZnSe and ZnSe-TiO 2 samples, as resulted from the UV-visible spectra of the collected supernatants from lysozyme loading processes (Supplementary materials- Figure S5). Still, the loaded lysozyme appears to be active against S. aureus and M. lysodeikticus in dark condition (Figures 19 and 20) and against M. lysodeikticus under visible light irradiation (Figure 21b). For identical irradiation experiments, S. aureus appears to display a lower resistance to the immobilized lysozyme action (Figure 21a) than M. lysodeikticus. By comparing Figures 19-21, some differences can be depicted in the reactivity of the investigated samples relative to the same substrate. This can be due to the different experimental conditions: dark and dynamic regime (Figures 19 and 20) versus light irradiation and static regime ( Figure 21). For the light assisted tests, the ROS presence was clearly emphasized and proved to be in line with the literature that assesses their antibacterial effect, especially for the hydroxyl radical (•OH), which is known as powerful oxidizing agent. In the present work, Figure 17 proved that •OH is produced mainly by the ZnSe sample and much less by ZnSe-TiO 2 . Figure 18 illustrates the O 2 •− photogeneration by ZnSe and ZnSe-TiO 2 samples before and after lysozyme immobilization. Generally, the ROS generation over semiconductor-type materials under irradiation in an aerobic medium can be described as follows [30]: •− ) ads (on semiconductor surface); (O 2 •− ) ads + 2H + +e − → H 2 O 2 → 2•OH In aqueous media, water photolysis can be also a source of •OH: (iii) H 2 O + hυ → •OH For our study, to a variable extent, all these mechanisms can to be involved in ROS generation. By correlating these observations with Figure 21, it can be assumed that there is a significant contribution by the photogenerated ROS to the antibacterial activity of ZnSe and ZnSe-TiO 2 samples against S. aureus and M. lysodeikticus. The slight antibacterial activity of TiO 2 is probably due to other mechanisms. On the other hand, the lower antibacterial activity of TiO 2 against S. aureus ( Figure 19) than for M. lysodeikticus suggests the development of self-defense mechanism(s) of the bacteria. Different structural features of the cell wall and/or a better self-repair capacity of S. aureus relative to other bacteria may account for these discrepancies.
Overall, the findings support the favorable impact of lysozyme addition to inorganic carriers on microbial growth inhibition for the investigated systems.
The antibacterial activity of Lys/ZnSe and Lys/ZnSe-TiO 2 systems is very high and quite similar. In our previous work [17], the enzymatic activity of these hybrid systems relative to a synthetic substrate was slightly higher for Lys/ZnSe-TiO 2 . This comparison indicates presumable differences between the antibacterial activity of lysozyme-derived systems and the enzymatic activity.

Conclusions
The antibacterial assays involving S. aureus and M. lysodeikticus showed very good results, both for the bare and most of the lysozyme-modified samples in the dark and when assisted by visible light irradiation.
Bacterial reduction for S. aureus (in dark) over unmodified samples was highest in the case of the ZnSe sample. The lysozyme-loaded ZnSe-TiO 2 and TiO 2 samples proved to have a better activity than the samples without lysozyme. This was emphasized also by Dark field microscopy characterization that illustrates the direct contact between Lys/ZnSe-TiO 2 and S. aureus.
Unmodified ZnSe-TiO 2 and ZnSe samples proved to be very efficient against M. lysodeikticus (in dark), with the lysozyme loading being beneficial for all samples, especially for TiO 2 .
For S. aureus, 100% bacterial reduction was obtained after exposing the ZnSe, ZnSe-TiO 2 , Lys/ZnSe and Lys/ZnSe-TiO 2 samples to visible light for 10 min. Also, the light exposure proved to be beneficial for enhancing the antibacterial activity of ZnSe, ZnSe-TiO 2 and TiO 2 against M. lysodeikticus before and after lysozyme loading.
These newly designed light sensitive materials are able to develop lysozyme-based hybrid complexes acting as efficient antibacterial agents under visible light exposure and in the dark.
Supplementary Materials: The following supporting information can be downloaded at: https: //www.mdpi.com/article/10.3390/antiox12030691/s1, Figure S1: The spectrum of the illumination source with cut off filter λ>420 nm; Figure S2